# Flory-Huggins solution theory

﻿
Flory-Huggins solution theory

Flory-Huggins solution theory is a mathematical model of the thermodynamics of polymer solutions which takes account of the great dissimilarity in molecular sizes in adapting the usual expression for the entropy of mixing. The result is an equation for the Gibbs free energy change $Delta G_m$ for mixing a polymer with a solvent. Although it makes simplifying assumptions, it generates useful results for interpreting experiments. The thermodynamic equation for the Gibbs free energy change accompanying mixing at constant temperature and (external) pressure is

:$Delta G_m = Delta H_m - TDelta S_m ,$

A change, denoted by $Delta$, is the value of a variable for a solution or mixture minus the values for the pure components considered separately. The objective is to find explicit formulas for $Delta H_m$ and $Delta S_m$, the enthalpy and entropy increments associated with the mixing process.

The result obtained by FloryRef|1 and HugginsRef|2 is

:$Delta G_m = RT \left[,n_1lnphi_1 + n_2lnphi_2 + n_1phi_2chi_\left\{12\right\},\right] ,$

The right-hand side is a function of the number of moles $n_1$ and volume fraction $phi_1$ of solvent (component $1$), the number of moles $n_2$ and volume fraction $phi_2$ of polymer (component $2$), with the introduction of a parameter chi $chi$ to take account of the energy of interdispersing polymer and solvent molecules. $R$ is the gas constant and $T$ is the absolute temperature. The volume fraction is analogous to the mole fraction, but is weighted to take account of the relative sizes of the molecules. For a small solute, the mole fractions would appear instead, and this modification is the innovation due to Flory and Huggins.

Derivation

We first calculate the "entropy" of mixing, the increase in the uncertainty about the locations of the molecules when they are interspersed. In the pure condensed phasessolvent and polymer — everywhere we look we find a molecule.Ref|3 Of course, any notion of "finding" a molecule in a given location is a thought experiment since we can't actually examine spatial locations the size of molecules. The expression for the entropy of mixing of small molecules in terms of mole fractions is no longer reasonable when the solute is a macromolecular chain. We take account of this dissymmetry in molecular sizes by assuming that individual polymer segments and individual solvent molecules occupy sites on a . Each site is occupied by exactly one molecule of the solvent or by one monomer of the polymer chain, so the total number of sites is

:$N = N_1 + xN_2,$

$N_1$ is the number of solvent molecules and $N_2$ is the number of polymer molecules, each of which has $x$ segments.Ref|4

From statistical mechanics we can calculate the entropy change, the increase in spatial uncertainty, as a result of mixing solute and solvent.

:$Delta S_m = -k \left[,N_1ln\left(N_1/N\right) + N_2ln\left(xN_2/N\right),\right] ,$

where $k$ is Boltzmann's constant. Define the lattice "volume fractions" $phi_1$ and $phi_2$

:$phi_1 = N_1/N,$ :$phi_2 = xN_2/N,$

These are also the probabilities that a given lattice site, chosen at random, is occupied by a solvent molecule or a polymer segment, respectively. Thus

:$Delta S_m = -k \left[,N_1lnphi_1 + N_2lnphi_2,\right] ,$

For a small solute whose molecules occupy just one lattice site, $x$ equals one, the volume fractions reduce to molecular or mole fractions, and we recover the usual equation from ideal mixing theory.

In addition to the entropic effect, we can expect an "enthalpy" change.Ref|5 There are three molecular interactions to consider: solvent-solvent $w_\left\{11\right\}$, monomer-monomer $w_\left\{22\right\}$ (not the covalent bonding, but between different chain sections), and monomer-solvent $w_\left\{12\right\}$. Each of the last occurs at the expense of the average of the other two, so the energy increment per monomer-solvent contact is

:

The total number of such contacts is

:$xN_2zphi_1 = N_1phi_2z,$

where $z$ is the coordination number, the number of nearest neighbors for a lattice site, each one occupied either by one chain segment or a solvent molecule. That is, $xN_2$ is the total number of polymer segments (monomers) in the solution, so $xN_2z$ is the number of nearest-neighbor sites to "all" the polymer segments. Multiplying by the probability $phi_1$ that any such site is occupied by a solvent molecule,Ref|6 we obtain the total number of polymer-solvent molecular interactions. An approximation following mean field theory is made by following this procedure, thereby reducing the complex problem of many interactions to a simpler problem of one interaction.

The enthalpy change is equal to the energy change per polymer monomer-solvent interaction multiplied by the number of such interactions

:$Delta H_m = N_1phi_2zDelta w,$

The polymer-solvent interaction parameter "chi" is defined as

:$chi_\left\{12\right\} = zDelta w/kT ,$

It depends on the nature of both the solvent and the solute, and is the only "material-specific" parameter in the model. The enthalpy change becomes

:$Delta H_m = k T N_1phi_2chi_\left\{12\right\} ,$

Assembling terms, the total free energy change is

:$Delta G_m = RT \left[,n_1lnphi_1 + n_2lnphi_2 + n_1phi_2chi_\left\{12\right\},\right] ,$

where we have converted the expression from molecules $N_1$ and $N_2$ to moles $n_1$ and $n_2$ by transferring Avogadro's number $N_A$ to the gas constant $R = kN_A$.

The value of the interaction parameter can be estimated from the Hildebrand solubility parameters $delta_a$ and $delta_b$

:$chi_\left\{12\right\} = V_\left\{seg\right\}\left(delta_a - delta_b\right)^2/RT ,$

where $V_\left\{seg\right\}$ is the actual volume of a polymer segment.

This treatment does not attempt to calculate the conformational entropy of folding for polymer chains. (See the random coil discussion.) The conformations of even amorphous polymers will change when they go into solution, and most thermoplastic polymers also have lamellar crystalline regions which do not persist in solution as the chains separate. These events are accompanied by additional entropy and energy changes.

More advanced models exist, such as the Flory-Krigbaum theory.

* [http://www.informit.com/content/images/chap3_0130181684/elementLinks/chap3_0130181684.pdf "Conformations, Solutions and Molecular Weight" (book chapter)] , Chapter 3 of Book Title: Polymer Science and Technology; by Joel R. Fried; 2nd Edition, 2003
* [http://www.composite-agency.com/materials-forum.htm Flory-Huggins in practice: discussion on solubility in polymer based materials]

References and footnotes

# "Thermodynamics of High Polymer Solutions," Paul J. Flory "Journal of Chemical Physics," August 1941, Volume 9, Issue 8, p. 660 [http://link.aip.org/getabs/servlet/GetabsServlet?prog=normal&id=JCPSA6000009000008000660000002&idtype=cvips&gifs=Yes Abstract] . Flory suggested that Huggins' name ought to be first since he had published several months earlier: Flory, P.J., "Thermodynamics of high polymer solutions," "J. Chem. Phys." 10:51-61 (1942) [http://www.garfield.library.upenn.edu/classics1985/A1985AFW3100001.pdf "Citation Classic" No. 18, May 6, 1985]
# "Solutions of Long Chain Compounds," Maurice L. Huggins "Journal of Chemical Physics," May 1941 Volume 9, Issue 5, p. 440 [http://link.aip.org/getabs/servlet/GetabsServlet?prog=normal&id=JCPSA6000009000005000440000001&idtype=cvips&gifs=yes Abstract]
# We are ignoring the "free volume" due to molecular disorder in liquids and amorphous solids as compared to crystals. This, and the assumption that monomers and solute molecules are really the same size, are the main "geometric" approximations in this model.
# For a real synthetic polymer, there is a statistical distribution of chain lengths, so $x$ would be an average.
# The enthalpy is the internal energy corrected for any pressure-volume work at constant (external) $P$. We are not making any distinction here. This allows the approximation of Helmholtz free energy, which is the natural form of free energy from the Flory-Huggins lattice theory, to Gibbs free energy.
# In fact, two of the sites adjacent to a polymer segment are occupied by other polymer segments since it is part of a chain; and one more, making three, for branching sites, but only one for terminals.

Wikimedia Foundation. 2010.

### Look at other dictionaries:

• Huggins — refers to:People with the surname Huggins: *Bob Huggins (born 1953), American college basketball coach *Charles Brenton Huggins (1901–1997), Canadian born American physician, physiologist, and cancer researcher *Godfrey Huggins, 1st Viscount… …   Wikipedia

• Flory, Paul J. — ▪ American chemist Introduction in full  Paul John Flory  born June 19, 1910, Sterling, Ill., U.S. died Sept. 8, 1985, Big Sur, Calif.       American polymer chemist who was awarded the 1974 Nobel Prize for Chemistry “for his fundamental… …   Universalium

• Maurice Loyal Huggins — (19 September 1897 17 December 1981) was a scientist who independently conceived the idea of hydrogen bonding and who was an early advocate for their role in stabilizing protein secondary structure. An important polymer theory, Flory Huggins… …   Wikipedia

• Paul Flory — Infobox Scientist name = Paul John Flory imagesize = 180px birth date = birth date|1910|6|19|mf=y birth place = Sterling, Illinois death date = death date and age|1985|9|9|1910|6|19 death place = Big Sur, California nationality = United States… …   Wikipedia

• Mean field theory — (MFT, also known as self consistent field theory) is a method to analyse physical systems with multiple bodies. A many body system with interactions is generally very difficult to solve exactly, except for extremely simple cases (random field… …   Wikipedia

• Polymere — Polymère Polymère est un mot qui vient du grec « pollus » plusieurs, et « meros » partie. Un polymère est une macromolécule, organique ou inorganique, constituée de l enchaînement répété d un même motif, le monomère (du grec… …   Wikipédia en Français

• Polymère — Fibres de polyester observées au MEB …   Wikipédia en Français

• Polymères — Polymère Polymère est un mot qui vient du grec « pollus » plusieurs, et « meros » partie. Un polymère est une macromolécule, organique ou inorganique, constituée de l enchaînement répété d un même motif, le monomère (du grec… …   Wikipédia en Français

• Флори, Пол Джон — В Википедии есть статьи о других людях с такой фамилией, см. Флори. Пол Джон Флори англ. Paul John Flory …   Википедия

• Polymer — Appearance of real linear polymer chains as recorded using an atomic force microscope on surface under liquid medium. Chain contour length for this polymer is 204 nm; thickness is 0.4 nm.[1] A polymer is a large molecule (macromolecule …   Wikipedia